# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1539260'
_audit_update_record             
;
2017-03-21 deposited with the CCDC.
2017-08-15 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C0 H110 Co4 K2 N0 O123 W19 Zn5'
_chemical_formula_weight         6212.80

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   C2/c

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   32.285
_cell_length_b                   14.674
_cell_length_c                   21.768
_cell_angle_alpha                90.00
_cell_angle_beta                 95.18
_cell_angle_gamma                90.00
_cell_volume                     10270.6
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    7323
_cell_measurement_theta_min      2.36
_cell_measurement_theta_max      27.91

_exptl_crystal_description       block
_exptl_crystal_colour            purple
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.18
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.018
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             11184
_exptl_absorpt_coefficient_mu    23.169
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.0651
_exptl_absorpt_correction_T_max  0.1029
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            26009
_diffrn_reflns_av_R_equivalents  0.0472
_diffrn_reflns_av_sigmaI/netI    0.0531
_diffrn_reflns_limit_h_min       -38
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_theta_min         1.27
_diffrn_reflns_theta_max         25.00
_reflns_number_total             9054
_reflns_number_gt                7477
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0488P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   no
_refine_ls_hydrogen_treatment    ?
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         9054
_refine_ls_number_parameters     694
_refine_ls_number_restraints     30
_refine_ls_R_factor_all          0.0452
_refine_ls_R_factor_gt           0.0337
_refine_ls_wR_factor_ref         0.0934
_refine_ls_wR_factor_gt          0.0839
_refine_ls_goodness_of_fit_ref   1.045
_refine_ls_restrained_S_all      1.044
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.186435(15) -0.45745(3) 0.57951(2) 0.01180(12) Uani 1 1 d . . .
W2 W 0.050525(15) -0.20762(3) 0.45872(2) 0.01212(12) Uani 1 1 d . . .
W3 W 0.352397(16) -0.03623(3) 0.56517(2) 0.01367(12) Uani 1 1 d . . .
W4 W 0.162149(16) -0.04511(3) 0.58890(2) 0.01429(12) Uani 1 1 d . . .
W5 W 0.120813(15) -0.05720(3) 0.42225(2) 0.01237(12) Uani 1 1 d . . .
W6 W 0.093169(16) -0.19556(3) 0.62466(2) 0.01435(12) Uani 1 1 d . . .
W7 W 0.086746(15) -0.41875(3) 0.54423(2) 0.01415(12) Uani 1 1 d . . .
W8 W 0.193375(15) -0.23030(3) 0.66051(2) 0.01166(12) Uani 1 1 d . . .
W9 W 0.114690(15) -0.24999(3) 0.35097(2) 0.01186(12) Uani 1 1 d . . .
W10 W 0.25346(2) -0.15456(5) 0.53449(3) 0.01240(16) Uani 0.50 1 d P . 1
Zn1 Zn 0.34109(4) -0.25068(8) 0.49602(5) 0.0094(3) Uani 1 1 d . . .
Zn2 Zn 0.28295(5) -0.33487(10) 0.60571(7) 0.0251(4) Uani 1 1 d . . .
Zn3 Zn 0.25346(2) -0.15456(5) 0.53449(3) 0.01240(16) Uani 0.50 1 d P . 2
Co2 Co 0.07342(6) -0.30731(12) 0.18644(7) 0.0206(4) Uani 1 1 d . . .
Co1 Co 0.09080(6) 0.18023(12) 0.36164(8) 0.0287(5) Uani 1 1 d . . .
K1 K 0.25589(8) -0.17813(16) 0.82833(11) 0.0151(5) Uani 1 1 d . . .
O1 O 0.3469(2) -0.3096(5) 0.4185(3) 0.0102(17) Uani 1 1 d . . .
O2 O 0.0538(3) -0.1852(6) 0.6727(3) 0.022(2) Uani 1 1 d . . .
O3 O 0.3537(3) 0.0528(5) 0.6159(4) 0.022(2) Uani 1 1 d . . .
O4 O -0.0028(3) -0.2087(5) 0.4592(3) 0.0170(18) Uani 1 1 d . . .
O5 O 0.1106(3) -0.0691(5) 0.6290(3) 0.0158(18) Uani 1 1 d . . .
O6 O 0.0630(3) -0.3321(5) 0.4907(4) 0.021(2) Uani 1 1 d . . .
O7 O 0.1784(2) -0.5298(5) 0.5055(3) 0.0144(18) Uani 1 1 d . . .
O8 O 0.0440(3) -0.4797(6) 0.5657(4) 0.023(2) Uani 1 1 d . . .
O9 O 0.0961(3) -0.2782(5) 0.2753(3) 0.0194(19) Uani 1 1 d . . .
O10 O 0.3812(2) -0.3013(5) 0.5564(3) 0.0110(17) Uani 1 1 d . . .
O11 O 0.2192(3) -0.2424(5) 0.7332(3) 0.021(2) Uani 1 1 d . . .
O12 O 0.1062(3) 0.0520(6) 0.3972(4) 0.023(2) Uani 1 1 d . . .
O13 O 0.1689(3) 0.0689(6) 0.6090(4) 0.023(2) Uani 1 1 d . . .
O14 O 0.0970(3) -0.4981(5) 0.4741(3) 0.0170(18) Uani 1 1 d . . .
O15 O 0.0910(2) -0.3255(5) 0.6071(3) 0.0134(17) Uani 1 1 d . . .
O16 O 0.3001(3) -0.0905(5) 0.5762(4) 0.0191(19) Uani 1 1 d . . .
O17 O 0.2385(3) -0.2243(5) 0.6108(4) 0.0159(18) Uani 1 1 d . . .
O18 O 0.0661(3) -0.1787(5) 0.5467(3) 0.0182(19) Uani 1 1 d . . .
O19 O 0.2090(3) -0.5394(5) 0.6289(4) 0.0181(19) Uani 1 1 d . . .
O20 O 0.1286(3) -0.4865(5) 0.5954(3) 0.0150(17) Uani 1 1 d U . .
O21 O 0.2115(3) -0.0650(5) 0.5479(3) 0.020(2) Uani 1 1 d . . .
O22 O 0.1048(3) -0.1206(5) 0.3438(3) 0.0125(17) Uani 1 1 d . . .
O23 O 0.3802(3) -0.1285(5) 0.6118(3) 0.0173(19) Uani 1 1 d . . .
O24 O 0.2862(2) -0.2706(5) 0.5230(3) 0.0096(16) Uani 1 1 d U . .
O25 O 0.1921(3) -0.0967(5) 0.6617(3) 0.0136(17) Uani 1 1 d . . .
O26 O 0.0591(3) -0.0870(5) 0.4403(3) 0.0182(19) Uani 1 1 d . . .
O27 O 0.0540(3) -0.2543(5) 0.3793(3) 0.0161(18) Uani 1 1 d U . .
O28 O 0.1745(3) -0.0632(5) 0.4110(3) 0.0171(18) Uani 1 1 d . . .
O29 O 0.2330(3) -0.4008(5) 0.5476(3) 0.0175(19) Uani 1 1 d . . .
O30 O 0.1852(2) -0.3549(5) 0.6360(3) 0.0123(17) Uani 1 1 d . . .
O31 O 0.1306(3) -0.0353(5) 0.5102(3) 0.0137(18) Uani 1 1 d . . .
O32 O 0.1367(3) -0.2269(5) 0.6887(3) 0.0169(18) Uani 1 1 d . . .
O33 O 0.1691(2) -0.2405(5) 0.3483(3) 0.0125(17) Uani 1 1 d . . .
O34 O 0.3536(2) -0.1238(5) 0.4843(3) 0.0126(17) Uani 1 1 d . . .
O1W O 0.2726(3) -0.3901(5) 0.6909(3) 0.021(2) Uani 1 1 d . . .
O2W O 0.0822(5) 0.3164(8) 0.3278(6) 0.072(4) Uani 1 1 d . . .
O3W O 0.1278(4) 0.1424(9) 0.2929(5) 0.064(4) Uani 1 1 d U . .
O4W O 0.0398(4) 0.1393(9) 0.3015(5) 0.066(4) Uani 1 1 d . . .
O5W O 0.1418(3) 0.2298(7) 0.4175(5) 0.047(3) Uani 1 1 d . . .
O6W O 0.0508(4) 0.2046(7) 0.4286(5) 0.046(3) Uani 1 1 d . . .
O7W O 0.1292(3) -0.3736(7) 0.1756(4) 0.040(3) Uani 1 1 d . . .
O8W O 0.0974(3) -0.1840(7) 0.1577(5) 0.039(3) Uani 1 1 d . . .
O9W O 0.0164(3) -0.2433(8) 0.1939(4) 0.042(3) Uani 1 1 d . . .
O10W O 0.0491(4) -0.4324(7) 0.2145(5) 0.050(3) Uani 1 1 d . . .
O11W O 0.0552(3) -0.3384(6) 0.0924(4) 0.032(2) Uani 1 1 d . . .
O12W O 0.3068(3) -0.3032(6) 0.8018(4) 0.038(3) Uani 1 1 d . . .
O13W O 0.2103(3) -0.1167(6) 0.9111(4) 0.029(2) Uani 1 1 d . . .
O14W O 0.2970(3) -0.1257(6) 0.7429(4) 0.031(2) Uani 1 1 d . . .
O15W O 0.2895(3) -0.2288(6) 0.9263(4) 0.040(3) Uani 1 1 d . . .
O16W O 0.2156(4) -0.3099(7) 0.8572(5) 0.048(3) Uani 1 1 d . . .
O17W O 0.2054(3) -0.0636(6) 0.7835(4) 0.032(2) Uani 1 1 d . . .
O18W O 0.0899(7) -0.0330(14) 0.2371(9) 0.135(7) Uani 1 1 d U . .
O19W O 0.2494(3) -0.6051(6) 0.4676(4) 0.035(2) Uani 1 1 d . . .
O20W O 0.3696(4) -0.1886(7) 0.9729(5) 0.048(3) Uani 1 1 d . . .
O21W O 0.0327(4) 0.3830(8) 0.4417(6) 0.066(4) Uani 1 1 d . . .
O22W O -0.0334(4) -0.4519(9) 0.1587(5) 0.068(4) Uani 1 1 d . . .
O23W O 0.0770(5) -0.1120(10) 0.0406(5) 0.077(5) Uani 1 1 d . . .
O24W O 0.3009(5) 0.0581(7) 0.7361(5) 0.064(4) Uani 1 1 d . . .
O25W O 0.1122(5) 0.4183(8) 0.2289(5) 0.079(5) Uani 1 1 d . . .
O26W O -0.0118(6) 0.0190(12) 0.4275(9) 0.133(7) Uani 1 1 d . . .
O27W O -0.0033(7) 0.3532(13) 0.3066(11) 0.157(8) Uani 1 1 d . . .
O28W O -0.0045(13) -0.0394(17) 0.3128(12) 0.108(14) Uani 0.50 1 d P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O19 1.730(8) . ?
W1 O29 1.903(8) . ?
W1 O7 1.928(7) . ?
W1 O30 1.946(7) . ?
W1 O20 1.977(8) . ?
W1 O34 2.169(8) 7_546 ?
W2 O4 1.721(8) . ?
W2 O26 1.841(8) . ?
W2 O27 1.872(7) . ?
W2 O18 1.982(8) . ?
W2 O6 1.983(8) . ?
W2 O10 2.261(8) 7_546 ?
W3 O3 1.709(8) . ?
W3 O23 1.871(8) . ?
W3 O16 1.903(8) . ?
W3 O14 1.977(8) 7_546 ?
W3 O7 2.004(7) 7_546 ?
W3 O34 2.182(7) . ?
W4 O13 1.737(8) . ?
W4 O31 1.918(7) . ?
W4 O21 1.918(8) . ?
W4 O25 1.934(7) . ?
W4 O5 1.979(8) . ?
W4 O1 2.156(7) 7_546 ?
W5 O12 1.744(8) . ?
W5 O28 1.776(8) . ?
W5 O31 1.939(7) . ?
W5 O22 1.972(7) . ?
W5 O26 2.111(8) . ?
W5 O10 2.130(7) 7_546 ?
W5 W9 3.2240(6) . ?
W6 O2 1.724(8) . ?
W6 O18 1.854(8) . ?
W6 O5 1.940(8) . ?
W6 O32 1.944(8) . ?
W6 O15 1.945(7) . ?
W6 O1 2.226(7) 7_546 ?
W7 O8 1.744(8) . ?
W7 O6 1.844(8) . ?
W7 O15 1.931(7) . ?
W7 O20 1.945(8) . ?
W7 O14 1.972(8) . ?
W7 O34 2.168(8) 7_546 ?
W8 O11 1.729(8) . ?
W8 O17 1.893(8) . ?
W8 O30 1.916(7) . ?
W8 O25 1.962(7) . ?
W8 O32 1.981(8) . ?
W8 O1 2.143(7) 7_546 ?
W8 K1 4.083(2) . ?
W9 O9 1.750(8) . ?
W9 O33 1.768(8) . ?
W9 O22 1.929(7) . ?
W9 O23 1.960(8) 7_546 ?
W9 O27 2.106(8) . ?
W9 O10 2.145(7) 7_546 ?
W10 O21 1.927(9) . ?
W10 O16 1.930(8) . ?
W10 O24 2.030(7) 7_546 ?
W10 O24 2.030(7) . ?
W10 O17 2.045(8) . ?
W10 O29 2.046(8) 7_546 ?
W10 Zn2 3.1692(17) . ?
W10 Zn2 3.1736(16) 7_546 ?
W10 W10 3.1763(13) 7_546 ?
Zn1 O10 1.911(8) . ?
Zn1 O1 1.920(7) . ?
Zn1 O34 1.927(8) . ?
Zn1 O24 1.940(7) . ?
Zn2 O24 2.044(7) . ?
Zn2 O1W 2.077(7) . ?
Zn2 O28 2.084(8) 7_546 ?
Zn2 O33 2.085(8) 7_546 ?
Zn2 O17 2.176(8) . ?
Zn2 O29 2.182(8) . ?
Zn2 W10 3.1736(16) 7_546 ?
Co2 O9 2.051(8) . ?
Co2 O7W 2.079(10) . ?
Co2 O9W 2.087(10) . ?
Co2 O8W 2.087(10) . ?
Co2 O10W 2.108(10) . ?
Co2 O11W 2.128(8) . ?
Co1 O6W 2.064(10) . ?
Co1 O3W 2.074(12) . ?
Co1 O12 2.078(8) . ?
Co1 O5W 2.087(11) . ?
Co1 O4W 2.098(12) . ?
Co1 O2W 2.138(11) . ?
K1 O15W 2.420(10) . ?
K1 O16W 2.444(10) . ?
K1 O19 2.471(8) 4_556 ?
K1 O17W 2.478(10) . ?
K1 O11 2.478(8) . ?
K1 O14W 2.501(9) . ?
K1 O12W 2.564(10) . ?
K1 O13W 2.588(9) . ?
O1 W8 2.143(7) 7_546 ?
O1 W4 2.156(7) 7_546 ?
O1 W6 2.226(7) 7_546 ?
O7 W3 2.004(7) 7_546 ?
O10 W5 2.130(7) 7_546 ?
O10 W9 2.145(7) 7_546 ?
O10 W2 2.261(8) 7_546 ?
O14 W3 1.977(8) 7_546 ?
O19 K1 2.471(8) 4_546 ?
O23 W9 1.960(8) 7_546 ?
O24 Zn3 2.030(7) 7_546 ?
O24 W10 2.030(7) 7_546 ?
O28 Zn2 2.084(8) 7_546 ?
O29 Zn3 2.046(8) 7_546 ?
O29 W10 2.046(8) 7_546 ?
O33 Zn2 2.085(8) 7_546 ?
O34 W7 2.168(8) 7_546 ?
O34 W1 2.169(8) 7_546 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O19 W1 O29 103.2(4) . . ?
O19 W1 O7 98.9(3) . . ?
O29 W1 O7 89.3(3) . . ?
O19 W1 O30 100.1(3) . . ?
O29 W1 O30 87.3(3) . . ?
O7 W1 O30 160.9(3) . . ?
O19 W1 O20 95.3(4) . . ?
O29 W1 O20 161.5(3) . . ?
O7 W1 O20 88.2(3) . . ?
O30 W1 O20 89.1(3) . . ?
O19 W1 O34 166.9(3) . 7_546 ?
O29 W1 O34 88.4(3) . 7_546 ?
O7 W1 O34 74.9(3) . 7_546 ?
O30 W1 O34 86.3(3) . 7_546 ?
O20 W1 O34 73.3(3) . 7_546 ?
O4 W2 O26 100.4(4) . . ?
O4 W2 O27 98.4(4) . . ?
O26 W2 O27 97.3(3) . . ?
O4 W2 O18 99.3(3) . . ?
O26 W2 O18 88.6(3) . . ?
O27 W2 O18 159.9(3) . . ?
O4 W2 O6 99.3(4) . . ?
O26 W2 O6 158.8(4) . . ?
O27 W2 O6 87.7(3) . . ?
O18 W2 O6 80.4(3) . . ?
O4 W2 O10 171.5(3) . 7_546 ?
O26 W2 O10 75.2(3) . 7_546 ?
O27 W2 O10 75.2(3) . 7_546 ?
O18 W2 O10 87.9(3) . 7_546 ?
O6 W2 O10 86.3(3) . 7_546 ?
O3 W3 O23 102.7(4) . . ?
O3 W3 O16 102.1(4) . . ?
O23 W3 O16 90.9(4) . . ?
O3 W3 O14 96.4(4) . 7_546 ?
O23 W3 O14 92.5(3) . 7_546 ?
O16 W3 O14 160.0(3) . 7_546 ?
O3 W3 O7 96.2(4) . 7_546 ?
O23 W3 O7 161.1(3) . 7_546 ?
O16 W3 O7 85.1(3) . 7_546 ?
O14 W3 O7 85.3(3) 7_546 7_546 ?
O3 W3 O34 166.0(3) . . ?
O23 W3 O34 88.2(3) . . ?
O16 W3 O34 86.3(3) . . ?
O14 W3 O34 74.1(3) 7_546 . ?
O7 W3 O34 73.1(3) 7_546 . ?
O13 W4 O31 101.4(4) . . ?
O13 W4 O21 100.0(4) . . ?
O31 W4 O21 89.6(3) . . ?
O13 W4 O25 97.4(4) . . ?
O31 W4 O25 161.3(3) . . ?
O21 W4 O25 86.9(3) . . ?
O13 W4 O5 98.7(4) . . ?
O31 W4 O5 90.4(3) . . ?
O21 W4 O5 160.9(3) . . ?
O25 W4 O5 87.0(3) . . ?
O13 W4 O1 169.6(3) . 7_546 ?
O31 W4 O1 87.1(3) . 7_546 ?
O21 W4 O1 85.8(3) . 7_546 ?
O25 W4 O1 74.3(3) . 7_546 ?
O5 W4 O1 75.1(3) . 7_546 ?
O12 W5 O28 104.1(4) . . ?
O12 W5 O31 99.9(3) . . ?
O28 W5 O31 94.0(3) . . ?
O12 W5 O22 96.9(3) . . ?
O28 W5 O22 92.4(3) . . ?
O31 W5 O22 160.0(3) . . ?
O12 W5 O26 90.9(4) . . ?
O28 W5 O26 164.9(3) . . ?
O31 W5 O26 85.6(3) . . ?
O22 W5 O26 83.4(3) . . ?
O12 W5 O10 162.0(4) . 7_546 ?
O28 W5 O10 91.8(3) . 7_546 ?
O31 W5 O10 87.2(3) . 7_546 ?
O22 W5 O10 73.6(3) . 7_546 ?
O26 W5 O10 73.1(3) . 7_546 ?
O12 W5 W9 130.7(3) . . ?
O28 W5 W9 84.7(3) . . ?
O31 W5 W9 128.2(2) . . ?
O22 W5 W9 33.8(2) . . ?
O26 W5 W9 83.7(2) . . ?
O10 W5 W9 41.21(19) 7_546 . ?
O2 W6 O18 103.4(4) . . ?
O2 W6 O5 96.5(4) . . ?
O18 W6 O5 91.6(3) . . ?
O2 W6 O32 96.4(4) . . ?
O18 W6 O32 159.8(3) . . ?
O5 W6 O32 90.2(3) . . ?
O2 W6 O15 101.0(4) . . ?
O18 W6 O15 86.8(3) . . ?
O5 W6 O15 162.4(3) . . ?
O32 W6 O15 85.4(3) . . ?
O2 W6 O1 165.7(3) . 7_546 ?
O18 W6 O1 88.0(3) . 7_546 ?
O5 W6 O1 74.2(3) . 7_546 ?
O32 W6 O1 73.2(3) . 7_546 ?
O15 W6 O1 88.2(3) . 7_546 ?
O8 W7 O6 103.3(4) . . ?
O8 W7 O15 100.4(4) . . ?
O6 W7 O15 87.6(3) . . ?
O8 W7 O20 96.3(4) . . ?
O6 W7 O20 160.4(4) . . ?
O15 W7 O20 87.5(3) . . ?
O8 W7 O14 95.5(3) . . ?
O6 W7 O14 90.4(3) . . ?
O15 W7 O14 164.0(3) . . ?
O20 W7 O14 89.1(3) . . ?
O8 W7 O34 165.9(3) . 7_546 ?
O6 W7 O34 87.1(3) . 7_546 ?
O15 W7 O34 89.5(3) . 7_546 ?
O20 W7 O34 73.9(3) . 7_546 ?
O14 W7 O34 74.5(3) . 7_546 ?
O11 W8 O17 101.3(4) . . ?
O11 W8 O30 101.5(3) . . ?
O17 W8 O30 88.8(3) . . ?
O11 W8 O25 95.7(3) . . ?
O17 W8 O25 88.8(3) . . ?
O30 W8 O25 162.7(3) . . ?
O11 W8 O32 95.9(4) . . ?
O17 W8 O32 162.7(3) . . ?
O30 W8 O32 90.2(3) . . ?
O25 W8 O32 87.1(3) . . ?
O11 W8 O1 165.9(3) . 7_546 ?
O17 W8 O1 88.3(3) . 7_546 ?
O30 W8 O1 88.8(3) . 7_546 ?
O25 W8 O1 74.1(3) . 7_546 ?
O32 W8 O1 74.4(3) . 7_546 ?
O11 W8 K1 16.7(3) . . ?
O17 W8 K1 99.2(2) . . ?
O30 W8 K1 118.2(2) . . ?
O25 W8 K1 79.1(2) . . ?
O32 W8 K1 96.5(2) . . ?
O1 W8 K1 151.91(19) 7_546 . ?
O9 W9 O33 104.2(4) . . ?
O9 W9 O22 96.7(3) . . ?
O33 W9 O22 94.5(3) . . ?
O9 W9 O23 100.6(3) . 7_546 ?
O33 W9 O23 92.2(3) . 7_546 ?
O22 W9 O23 159.4(3) . 7_546 ?
O9 W9 O27 91.1(4) . . ?
O33 W9 O27 164.7(3) . . ?
O22 W9 O27 84.3(3) . . ?
O23 W9 O27 84.1(3) 7_546 . ?
O9 W9 O10 162.5(4) . 7_546 ?
O33 W9 O10 91.5(3) . 7_546 ?
O22 W9 O10 74.1(3) . 7_546 ?
O23 W9 O10 86.2(3) 7_546 7_546 ?
O27 W9 O10 73.5(3) . 7_546 ?
O9 W9 W5 131.4(3) . . ?
O33 W9 W5 86.0(2) . . ?
O22 W9 W5 34.7(2) . . ?
O23 W9 W5 126.9(2) 7_546 . ?
O27 W9 W5 84.5(2) . . ?
O10 W9 W5 40.87(19) 7_546 . ?
O21 W10 O16 97.2(3) . . ?
O21 W10 O24 92.9(3) . 7_546 ?
O16 W10 O24 167.1(3) . 7_546 ?
O21 W10 O24 166.0(3) . . ?
O16 W10 O24 94.3(3) . . ?
O24 W10 O24 77.0(3) 7_546 . ?
O21 W10 O17 89.8(3) . . ?
O16 W10 O17 95.3(3) . . ?
O24 W10 O17 92.7(3) 7_546 . ?
O24 W10 O17 81.0(3) . . ?
O21 W10 O29 94.0(3) . 7_546 ?
O16 W10 O29 89.9(3) . 7_546 ?
O24 W10 O29 81.3(3) 7_546 7_546 ?
O24 W10 O29 94.1(3) . 7_546 ?
O17 W10 O29 173.0(3) . 7_546 ?
O21 W10 Zn2 132.8(2) . . ?
O16 W10 Zn2 89.4(2) . . ?
O24 W10 Zn2 89.7(2) 7_546 . ?
O24 W10 Zn2 39.08(19) . . ?
O17 W10 Zn2 42.9(2) . . ?
O29 W10 Zn2 132.9(2) 7_546 . ?
O21 W10 Zn2 88.6(2) . 7_546 ?
O16 W10 Zn2 133.0(2) . 7_546 ?
O24 W10 Zn2 38.98(19) 7_546 7_546 ?
O24 W10 Zn2 89.5(2) . 7_546 ?
O17 W10 Zn2 131.5(2) . 7_546 ?
O29 W10 Zn2 43.0(2) 7_546 7_546 ?
Zn2 W10 Zn2 119.90(3) . 7_546 ?
O21 W10 W10 130.7(2) . 7_546 ?
O16 W10 W10 132.1(2) . 7_546 ?
O24 W10 W10 38.5(2) 7_546 7_546 ?
O24 W10 W10 38.5(2) . 7_546 ?
O17 W10 W10 86.0(2) . 7_546 ?
O29 W10 W10 87.0(2) 7_546 7_546 ?
Zn2 W10 W10 60.02(3) . 7_546 ?
Zn2 W10 W10 59.88(3) 7_546 7_546 ?
O10 Zn1 O1 108.4(3) . . ?
O10 Zn1 O34 109.2(3) . . ?
O1 Zn1 O34 106.3(3) . . ?
O10 Zn1 O24 108.3(3) . . ?
O1 Zn1 O24 111.3(3) . . ?
O34 Zn1 O24 113.2(3) . . ?
O24 Zn2 O1W 172.4(3) . . ?
O24 Zn2 O28 95.2(3) . 7_546 ?
O1W Zn2 O28 92.1(3) . 7_546 ?
O24 Zn2 O33 94.8(3) . 7_546 ?
O1W Zn2 O33 87.1(3) . 7_546 ?
O28 Zn2 O33 89.6(3) 7_546 7_546 ?
O24 Zn2 O17 77.7(3) . . ?
O1W Zn2 O17 94.9(3) . . ?
O28 Zn2 O17 172.7(3) 7_546 . ?
O33 Zn2 O17 92.6(3) 7_546 . ?
O24 Zn2 O29 77.8(3) . . ?
O1W Zn2 O29 100.1(3) . . ?
O28 Zn2 O29 92.5(3) 7_546 . ?
O33 Zn2 O29 172.4(3) 7_546 . ?
O17 Zn2 O29 84.5(3) . . ?
O24 Zn2 W10 38.8(2) . . ?
O1W Zn2 W10 134.2(2) . . ?
O28 Zn2 W10 133.4(2) 7_546 . ?
O33 Zn2 W10 88.2(2) 7_546 . ?
O17 Zn2 W10 39.8(2) . . ?
O29 Zn2 W10 85.0(2) . . ?
O24 Zn2 W10 38.7(2) . 7_546 ?
O1W Zn2 W10 139.8(3) . 7_546 ?
O28 Zn2 W10 89.4(2) 7_546 7_546 ?
O33 Zn2 W10 133.1(2) 7_546 7_546 ?
O17 Zn2 W10 84.1(2) . 7_546 ?
O29 Zn2 W10 39.8(2) . 7_546 ?
W10 Zn2 W10 60.10(3) . 7_546 ?
O9 Co2 O7W 88.0(4) . . ?
O9 Co2 O9W 94.3(4) . . ?
O7W Co2 O9W 177.6(4) . . ?
O9 Co2 O8W 89.5(4) . . ?
O7W Co2 O8W 91.3(4) . . ?
O9W Co2 O8W 89.2(4) . . ?
O9 Co2 O10W 91.1(4) . . ?
O7W Co2 O10W 88.6(5) . . ?
O9W Co2 O10W 90.8(4) . . ?
O8W Co2 O10W 179.4(4) . . ?
O9 Co2 O11W 175.1(4) . . ?
O7W Co2 O11W 87.5(4) . . ?
O9W Co2 O11W 90.2(4) . . ?
O8W Co2 O11W 88.5(4) . . ?
O10W Co2 O11W 90.8(4) . . ?
O6W Co1 O3W 173.9(5) . . ?
O6W Co1 O12 92.2(4) . . ?
O3W Co1 O12 83.9(4) . . ?
O6W Co1 O5W 92.2(5) . . ?
O3W Co1 O5W 92.2(5) . . ?
O12 Co1 O5W 87.1(4) . . ?
O6W Co1 O4W 89.1(5) . . ?
O3W Co1 O4W 86.8(5) . . ?
O12 Co1 O4W 96.9(4) . . ?
O5W Co1 O4W 175.7(5) . . ?
O6W Co1 O2W 90.6(4) . . ?
O3W Co1 O2W 93.8(5) . . ?
O12 Co1 O2W 173.5(5) . . ?
O5W Co1 O2W 86.9(5) . . ?
O4W Co1 O2W 89.0(5) . . ?
O15W K1 O16W 74.8(4) . . ?
O15W K1 O19 76.6(3) . 4_556 ?
O16W K1 O19 142.4(3) . 4_556 ?
O15W K1 O17W 141.4(3) . . ?
O16W K1 O17W 106.9(4) . . ?
O19 K1 O17W 81.5(3) 4_556 . ?
O15W K1 O11 139.6(3) . . ?
O16W K1 O11 71.9(3) . . ?
O19 K1 O11 142.8(3) 4_556 . ?
O17W K1 O11 71.4(3) . . ?
O15W K1 O14W 121.6(4) . . ?
O16W K1 O14W 139.9(3) . . ?
O19 K1 O14W 76.7(3) 4_556 . ?
O17W K1 O14W 82.7(3) . . ?
O11 K1 O14W 75.0(3) . . ?
O15W K1 O12W 74.5(3) . . ?
O16W K1 O12W 81.9(4) . . ?
O19 K1 O12W 113.1(3) 4_556 . ?
O17W K1 O12W 143.9(3) . . ?
O11 K1 O12W 78.9(3) . . ?
O14W K1 O12W 70.0(3) . . ?
O15W K1 O13W 74.4(3) . . ?
O16W K1 O13W 75.4(3) . . ?
O19 K1 O13W 73.8(3) 4_556 . ?
O17W K1 O13W 69.1(3) . . ?
O11 K1 O13W 117.1(3) . . ?
O14W K1 O13W 141.6(3) . . ?
O12W K1 O13W 145.3(3) . . ?
O15W K1 W8 151.2(2) . . ?
O16W K1 W8 81.4(3) . . ?
O19 K1 W8 131.6(2) 4_556 . ?
O17W K1 W8 61.4(2) . . ?
O11 K1 W8 11.58(18) . . ?
O14W K1 W8 69.2(2) . . ?
O12W K1 W8 86.5(2) . . ?
O13W K1 W8 114.9(2) . . ?
Zn1 O1 W8 118.8(4) . 7_546 ?
Zn1 O1 W4 119.2(3) . 7_546 ?
W8 O1 W4 98.1(3) 7_546 7_546 ?
Zn1 O1 W6 120.9(4) . 7_546 ?
W8 O1 W6 98.0(3) 7_546 7_546 ?
W4 O1 W6 96.9(3) 7_546 7_546 ?
W6 O5 W4 113.6(4) . . ?
W7 O6 W2 156.4(5) . . ?
W1 O7 W3 113.3(4) . 7_546 ?
W9 O9 Co2 178.2(5) . . ?
Zn1 O10 W5 119.8(4) . 7_546 ?
Zn1 O10 W9 119.4(4) . 7_546 ?
W5 O10 W9 97.9(3) 7_546 7_546 ?
Zn1 O10 W2 119.1(3) . 7_546 ?
W5 O10 W2 97.9(3) 7_546 7_546 ?
W9 O10 W2 98.0(3) 7_546 7_546 ?
W8 O11 K1 151.7(4) . . ?
W5 O12 Co1 175.9(5) . . ?
W7 O14 W3 112.8(4) . 7_546 ?
W7 O15 W6 146.4(4) . . ?
W3 O16 W10 143.9(4) . . ?
W8 O17 W10 137.6(4) . . ?
W8 O17 Zn2 122.6(4) . . ?
W10 O17 Zn2 97.3(3) . . ?
W6 O18 W2 156.0(5) . . ?
W1 O19 K1 163.7(4) . 4_546 ?
W7 O20 W1 114.1(4) . . ?
W4 O21 W10 143.0(4) . . ?
W9 O22 W5 111.5(3) . . ?
W3 O23 W9 154.3(5) . 7_546 ?
Zn1 O24 Zn3 115.9(3) . 7_546 ?
Zn1 O24 W10 115.9(3) . 7_546 ?
Zn3 O24 W10 0.00(6) 7_546 7_546 ?
Zn1 O24 W10 114.3(3) . . ?
Zn3 O24 W10 103.0(3) 7_546 . ?
W10 O24 W10 103.0(3) 7_546 . ?
Zn1 O24 Zn2 117.2(4) . . ?
Zn3 O24 Zn2 102.4(3) 7_546 . ?
W10 O24 Zn2 102.4(3) 7_546 . ?
W10 O24 Zn2 102.1(3) . . ?
W4 O25 W8 112.9(4) . . ?
W2 O26 W5 113.7(4) . . ?
W2 O27 W9 113.3(4) . . ?
W5 O28 Zn2 136.6(4) . 7_546 ?
W1 O29 Zn3 136.9(4) . 7_546 ?
W1 O29 W10 136.9(4) . 7_546 ?
Zn3 O29 W10 0.00(4) 7_546 7_546 ?
W1 O29 Zn2 123.3(4) . . ?
Zn3 O29 Zn2 97.2(3) 7_546 . ?
W10 O29 Zn2 97.2(3) 7_546 . ?
W8 O30 W1 154.7(4) . . ?
W4 O31 W5 153.6(5) . . ?
W6 O32 W8 114.4(4) . . ?
W9 O33 Zn2 136.3(4) . 7_546 ?
Zn1 O34 W7 121.3(4) . 7_546 ?
Zn1 O34 W1 119.7(4) . 7_546 ?
W7 O34 W1 98.7(3) 7_546 7_546 ?
Zn1 O34 W3 116.3(3) . . ?
W7 O34 W3 98.2(3) 7_546 . ?
W1 O34 W3 98.0(3) 7_546 . ?

_diffrn_measured_fraction_theta_max 1.000
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 1.000
_refine_diff_density_max         2.670
_refine_diff_density_min         -2.404
_refine_diff_density_rms         0.414
